- Research article
- Open Access
Experimental and theoretical studies of Schiff bases as corrosion inhibitors
© The Author(s) 2018
- Received: 20 April 2017
- Accepted: 20 January 2018
- Published: 5 February 2018
Relatively inexpensive, stable Schiff bases, namely 3-((4-hydroxybenzylidene)amino)-2-methylquinazolin-4(3H)-one (BZ3) and 3-((4-(dimethylamino)benzylidene)amino)-2-methylquinazolin-4(3H)-one (BZ4), were employed as highly efficient inhibitors of mild steel corrosion by corrosive acid.
The inhibition efficiencies were estimated based on weight loss method. Moreover, scanning electron microscopy was used to investigate the inhibition mechanism. The synthesized Schiff bases were characterized by Fourier transform infrared spectroscopy, nuclear magnetic resonance spectroscopy and micro-elemental analysis. The inhibition efficiency depends on three factors: the amount of nitrogen in the inhibitor, the inhibitor concentration and the inhibitor molecular weight.
Inhibition efficiencies of 96 and 92% were achieved with BZ4 and BZ3, respectively, at the maximum tested concentration. Density functional theory calculations of BZ3 and BZ4 were performed to compare the effects of hydroxyl and N,N-dimethylamino substituents on the inhibition efficiency, providing insight for designing new molecular structures that exhibit enhanced inhibition efficiencies.
- Schiff bases
- Corrosion inhibitors
Anti-corrosion coatings are generally employed to inhibit the average of corrosion and increase longevity of the mild steel. A broad range of organic adsorption inhibitors presently applied in the corrosion domain are expensive [1, 2]. Electron pairs and negative ions are transferred from the inhibitors to the metal d orbitals, resulting in the formation of coordination complexes with specific geometries, such as square planar, tetrahedral or octahedral . Thus, inhibitor molecules improve mild steel resistance to corrosive solutions by adsorbing on the metal surface [4–7] and forming a barrier that blocks the mild steel active sites [8–10]. Inhibitor adsorption on mild steel is affected by the nature of the mild steel, type of electrolyte and molecular structure of the inhibitor [11, 12]. Inhibitors molecules adsorbed on surface of mild steel, forming a barrier and consequently preventing reactions (cathodic or anodic) from processing at the surface of mild steel. These inhibitors could react with the iron atom at the mild steel surface to form in-organic complexes, blocking the surface of mild steel . Quantum chemical investigations have extensively been employed for correlating the inhibitor molecular structures and the inhibition impacts . To extend our previous work on designing novel inhibitor molecules [15–24], the Schiff bases 3-((4-hydroxybenzylidene)amino)-2-methylquinazolin-4(3H)-one (BZ3) and 3-((4-(dimethylamino)benzylidene)amino)-2-methylquinazolin-4(3H)-one (BZ4) were synthesized. Their molecular structures were determined by elemental analysis; carbon, hydrogen and nitrogen (mass fractions of CHN) analysis, Fourier transform infrared FTIR spectroscopy and nuclear magnetic resonance (NMR) spectroscopy. The abilities of these molecules to inhibit mild steel corrosion in an acidic solution were determined by the weight loss method and scanning electron microscopy (SEM). To elucidate the inhibition mechanism and the relationship between the structure and inhibition efficiency of the inhibitor, quantum chemical calculations of BZ3 and BZ4 were performed.
All chemical compounds were purchased from Sigma-Aldrich/Malaysia. Fourier transform infrared (FTIR) spectra were recorded on a Shimadzu FTIR-8300 spectrometer. Elemental analyses were performed using a Carlo Erba 5500 elemental analysis; carbon, hydrogen and nitrogen (CHN). Nuclear magnetic resonance spectra were obtained using a Bruker Spectrospin instrument equipped with 300 MHz UltraShield magnets. DMSO-d6 and TMS were used as the solvent and internal standard, respectively.
Synthesis of corrosion inhibitors
An ethanolic solution of 3-amino-2-methylquinazolin-4(3H)-one (0.005 mol), the appropriate carbonyl compound (0.005 mol) and a few drops of acetic acid were refluxed for 8 h. After cooling, the mixture was filtered, and the obtained solid was subsequently washed and recrystallized from hot ethanol. BZ3: yield 72%, mp 204–206 °C. FTIR: 3189 (br, aromatic O–H), 1704.3 (C=O), 1609.0 (C=N). 1H NMR: 2.37 (s, 3H, CH3), 6.84–7.01 (m, 1H, Ar–H), 5.32 (s, 1H, OH), 9.33 (d, 1H, H–C=N). Elemental analysis (CHN): C 69.11% (68.81%), H 4.91% (4.69%), N 14.82 (15.05). BZ4: yield 68%, mp 191–193 °C. FTIR: 3047.4 (aromatic C–H), 1699.6 (C=O), 1611.3 (C=N). 1H NMR: 2.410 (s, 3H, CH3), 7.01–7.32 (m, 1H, Ar–H), 8.99 (d, 1H, H–C=N). Elemental analysis (CHN): C 70.90% (70.57%), H 6.03% (5.92%), N 18.78 (18.29%).
Ground-state geometry optimizations were performed without symmetry constraints using Gaussian 09, Revision A.02 . The hybrid functional B3LYP was employed for all the geometry optimizations and highest occupied and lowest unoccupied molecular orbital energy calculations [29, 30].
Weight loss results
In industry, the use of inhibitors is one of the major economical methods for efficiently safeguarding mild steel surfaces against corrosion . Organic inhibitors are the predominant compounds used in the oil industry because they can act as a barrier for mild steel against corrosive media. Most of these inhibitors are heterocyclic molecules, such as pyridine, imidazoline and azoles [32–34], or polymers [35, 36].
Proposed inhibition mechanism
The inhibition mechanism of the tested inhibitors can be explained by valence bond theory (VBT). The Fe2+ electron configuration is [Ar]3d6. The 3d orbitals mix with the unoccupied 4s and 4p orbitals to form sp3 or d2sp3 hybrid orbitals that might be suitably oriented toward the nitrogen or oxygen non-bonding electron pairs in the inhibitors. When these Fe and inhibitor orbitals overlap, tetrahedral, square planar or octahedral complexes in which the metal has a filled valence shell are formed. The inhibition mechanism can also be explained in terms of crystal field theory (CFT) or molecular orbital theory (MOT). When the inhibitor molecules complex to the metal atoms, coordination bonds form via electron transfer from the inhibitor nitrogen atoms to the metal d orbitals.
Scanning electron microscopy
To elucidate the significant electronic effects of the substituents, the two inhibitors with strongly electron-donating groups, namely 3-((4-hydroxybenzylidene)amino)-2-methylquinazolin-4(3H)-one (BZ3) with a hydroxyl (–OH) group and 3-((4-(dimethylamino)benzylidene)amino)-2-methylquinazolin-4(3H)-one (BZ4) with an N,N-dimethylamino (–NMe2) group, were studied by DFT. Two additional isomer models of both BZ3 and BZ4 were also investigated .
Calculated HOMO and LUMO energies, energy gaps, ionization potentials, and electron affinities (eV) for BZ3, BZ3a and BZ3b obtained with rB3LYP/6-31G(d,p)
Energy gap (ELUMO − EHOMO)
Ionization potential (I)
Electron affinity (A)
I = − EHOMO; A = − ELUMO
Theoretical inhibition efficiencies (%) for BZ3, BZ3a and BZ3b
Inhibition efficiency (%)
Theoretical (Ie theory )
These results demonstrate that moving the hydroxyl group to the meta position (BZ3b) led to a decrease in the inhibition efficiency to 77.81%, whereas moving it to the ortho position (BZ3a) resulted in an increase in the inhibition efficiency to 96.11%. A comparison of the BZ3 and BZ3a inhibition efficiencies (96.11% vs. 92%) reveals that this change in the substituent position clearly enhanced the inhibition efficiency.
Calculated HOMO and LUMO energies, energy gaps, ionization potentials, and electron affinities (eV) for BZ4, BZ4a and BZ4b obtained with rB3LYP/6-31G(d,p)
Energy gap (ELUMO − EHOMO)
Ionization potential (I)
Electron affinity (A)
The ionization potential (I) and electron affinity (A) were calculated according to Koopmans’ theorem  as follows:
I = − EHOMO; A = − ELUMO
Theoretical inhibition efficiencies (%) for BZ4, BZ4a and BZ4b
Inhibition efficiency (%)
Theoretical (Ie theory )
These results demonstrate that moving the N,N-dimethylamino substituent to the meta position (BZ4b) led to a decrease in the inhibition efficiency to 85.27%, whereas moving it to the ortho position (BZ4a) resulted in an increase in the inhibition efficiency to 94.98%. This result along with that for BZ4 (96%) reveals that an excellent inhibition efficiency could be achieved with BZ4 isomers.
Groups which were withdrawing electron by resonance effect will decrease density of electrons specifically at positions 2, 4 and 6, leaving position 3 and position 5 as the ones with relatively higher efficiency, thus these kinds of groups were (position-3) meta directors. Also, the groups that have unoccupied pair of electrons, like the amino group (BZ4) or hydroxyl group (BZ3), are strong active and ortho (BZa)/para-directors (BZ) thus efficient groups donate the unoccupied electrons to the pi system, making a negative charge on ortho (position-2) and para (position-4)positions. These positions have the maximum activities toward electron-poor electrophile. The highest electron density have been located on ortho/para positions, although. An important point; steric hindrance as in compound BZ4 that have 2-methyl groups on nitrogen atom (N,N-dimethyl) decrease the reactivity. The final result of the electrophilic aromatic substitution might thus be hard to predict, and it is usually only established by doing the reaction and determining the ratio of ortho versus para substitution.
Mild steel corrosion inhibitors were synthesized, and their structures were fully characterized by spectroscopic techniques. Their abilities to inhibit mild steel corrosion in a 1.0 M HCl solution at 303, 313, 323 and 333 K were subsequently studied. The inhibitors, namely 3-((4-hydroxybenzylidene)amino)-2-methylquinazolin-4(3H)-one (BZ3) and 3-((4-(dimethylamino)benzylidene)amino)-2-methylquinazolin-4(3H)-one (BZ4), exhibited excellent corrosion inhibition performances, and maximum inhibition efficiencies of 96 and 92% were observed for BZ4 and BZ3, respectively, at an inhibitor concentration of 5 mM. The inhibition efficiency increased with increasing inhibitor concentration, whereas it decreased with increasing temperature. The SEM images show that BZ4 might form a protective film on the mild steel surface.
Quantum chemical calculations were performed to elucidate the relationship between the electronic structures of the inhibitors and their corrosion inhibition efficiencies. In particular, the rB3LYP/6-31G(d,p) calculations of BZ3 and BZ4 isomers revealed that a substituent in the meta position on the corrosion inhibitor molecule negatively affected the inhibition efficiency, whereas a substituent in the para position enhanced the inhibition efficiency. Compared to other corrosion inhibitors, these molecules exhibited higher inhibition efficiencies. The theoretical and experimental inhibition efficiencies of the studied inhibitors were in excellent agreement, demonstrating the reliability of the method employed.
DMA and SBA performed the synthesis of the corrosion inhibitors. AKA and AK evaluate the inhibition efficiency of the inhibitors as corrosion inhibitors. TSG measured the FT-IR and NMR spectra. AAHK and ABM characterized and they were the principle investigator. AAA write the manuscript. All authors read and approved the final manuscript.
The authors gratefully acknowledge the Universiti Kebangsaan Malaysia under Grant DIP-2012-02.
The authors declare that they have no competing interests.
Ethics approval and consent to participate
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.
- Ahamad I, Prasad R, Quraishi MA (2010) Thermodynamic, electrochemical and quantum chemical investigation of some Schiff bases as corrosion inhibitors for mild steel in hydrochloric acid solutions. Corros Sci 52:933–942View ArticleGoogle Scholar
- Amin MA, Khaled KF, Mohsen Q, Arida HA (2010) A study of the inhibition of iron corrosion in HCl solutions by some amino acids. Corros Sci 52:1684–1695View ArticleGoogle Scholar
- Anitha C, Sheela CD, Tharmaraj P, Shanmugakala R (2013) Studies on synthesis and spectral characterization of some transition metal complexes of azo-azomethine derivative of diaminomaleonitrile. Int J Inorg Chem 2013:1–10View ArticleGoogle Scholar
- Yıldırım A, Çetin M (2008) Synthesis and evaluation of new long alkyl side chain acetamide, isoxazolidine and isoxazoline derivatives as corrosion inhibitors. Corros Sci 50:155–165View ArticleGoogle Scholar
- Emregul KC, Hayvalı M (2004) Studies on the effect of vanillin and protocatechualdehyde on the corrosion of steel in hydrochloric acid. Mater Chem Phys 83:209–216View ArticleGoogle Scholar
- Solmaz R (2008) Investigation of adsorption and inhibitive effect of 2-mercaptothiazoline on corrosion of mild steel in hydrochloric acid media. Electrochim Acta 53:5941–5952View ArticleGoogle Scholar
- Bockris JO, Swinkels DAJ (1964) Adsorotion of naphthalene on solid metal electrodes. J Electrochem Soc 111:743–748View ArticleGoogle Scholar
- Branzoi V, Branzoi F, Baibarac M (2000) The inhibition of the corrosion of Armco iron in HCl solutions in the presence of surfactants of the type of N-alkyl quaternary ammonium salts. Mater Chem Phys 65:288–297View ArticleGoogle Scholar
- Oguzie EE, Li Y, Wang FH (2007) Corrosion inhibition and adsorption behavior of methionine on mild steel in sulfuric acid and synergistic effect of iodide ion. J Colloid Interface Sci 310:90–98View ArticleGoogle Scholar
- Alijourani J, Raeissi K, Golozar MA (2009) Benzimidazole and its derivatives as corrosion inhibitors for mild steel in 1 M HCl solution. Corros Sci 51:1836–1843View ArticleGoogle Scholar
- Obot IB, Obi-Egbedi NO (2010) Theoretical study of benzimidazole and its derivatives and their potential activity as corrosion inhibitors. Corros Sci 52:198–204View ArticleGoogle Scholar
- Li (2006) Synergistic inhibition between o-phenanthroline and chloride ion for steel corrosion in sulphuric acid. Corros Sci 48:308–321View ArticleGoogle Scholar
- Kadhum A, Mohamad AB, Hammed L, Al-Amiery AA, San NH (2014) Musa AY Inhibition of mild steel corrosion in hydrochloric acid solution by new coumarin. Materials 7:4335–4348View ArticleGoogle Scholar
- Xia S, Qiu M, Yu L, Liu F, Zhao H (2008) Molecular dynamics and density functional theory study on relationship between structure of imidazoline derivatives and inhibition performance. Corros Sci 50:2021–2029View ArticleGoogle Scholar
- Al-Amiery A, Al-Majedy Y, Kadhum A (2015) Hydrogen peroxide scavenging activity of novel coumarins synthesized using different approaches. PLoS ONE 10(7):e0132175View ArticleGoogle Scholar
- Al-Amiery AA, Al-Bayati R, Saour K, Radi M (2012) Cytotoxicity, antioxidant and antimicrobial activities of novel 2-quinolone derivatives derived from coumarins. Res Chem Intermed 38(2):559–569View ArticleGoogle Scholar
- Al-Amiery AA, Al-MajedyKadhum AAH, Mohamad A (2015) Novel macromolecules derived from coumarin: synthesis and antioxidant activity. Sci Rep 5:11825View ArticleGoogle Scholar
- Al-Amiery AA, Al-Majedy YK, Al-Duhaidahawi D, Kadhum AAH, Mohamad AB (2016) Green antioxidants: synthesis and scavenging activity of coumarin-thiadiazoles as potential antioxidants complemented by molecular modeling studies. Free Radic Antioxid 6(2):173–177View ArticleGoogle Scholar
- Al-Amiery AA, Al-Majedy YK, Kadhum AA, Mohamad AB (2014) New coumarin derivative as an eco-friendly inhibitor of corrosion of mild steel in acid medium. Molecules 20(1):366–383View ArticleGoogle Scholar
- Al-Amiery AA, Al-Majedy YK, Kadhum AAH, Mohamad AB (2016) Synthesis of new coumarins complemented by quantum chemical studies. Res Chem Intermed 42(4):3905–3918View ArticleGoogle Scholar
- Al-Amiery AA, Kadhum AAH, Mohamad AA (2012) Antifungal activities of new coumarins. Molecules 17(5):5713–5723View ArticleGoogle Scholar
- Al-Amiery AA, Kadhum AAH, Mohamad AB, Musa AY, Li CJ (2013) Electrochemical study on newly synthesized chlorocurcumin as an inhibitor for mild steel corrosion in hydrochloric acid. Materials 6(12):5466–5477View ArticleGoogle Scholar
- Al-Amiery AA, Musa AY, Kadhum A, Mohamad A (2011) The use of umbelliferone in the synthesis of new heterocyclic compounds. Molecules 16(8):6833–6843View ArticleGoogle Scholar
- Al-Majedy Y, Kadhum K, Al-Amiery AAH (2014) A synthesis and characterization of some new 4-hydroxy-coumarin derivatives. Molecules 19(8):11791–11799View ArticleGoogle Scholar
- American Society for Testing and Materials. Standard practice for preparing, cleaning, and evaluating corrosion test specimens. http://www.cosasco.com/documents/ASTM_G1_Standard_Practice.pdf. Accessed 11 Mar 2013
- Al-amiery AA, Abdul AHK, Abu BM, Sutiana J (2013) A novel hydrazinecarbothioamide as a potential corrosion inhibitor for mild steel in HCl. Materials 6:1420–1431View ArticleGoogle Scholar
- Junaedi S, Al-amiery A, Kadihum A, Mohamad A (2013) Inhibition effects of a synthesized novel 4-aminoantipyrine derivative on the corrosion of mild steel in hydrochloric acid solution together with quantum chemical studies. Int J Mol Sci 14:11915–11928View ArticleGoogle Scholar
- Ramarajan D, Tamilarasan K, Sudha S (2017) Synthesis, crystal structure analysis and DFT studies of 3a,8a-dihydroxy-2-thioxo-2,3,3a,8a-tetrahydroindeno[1,2-d] imidazol-8(1H)-one. J Mol Struct 1139(5):282–293View ArticleGoogle Scholar
- Pandey M, Muthu S, Gowda N (2017) Quantum mechanical and spectroscopic (FT-IR, FT-Raman,1H,13C NMR, UV–Vis) studies, NBO, NLO, HOMO, LUMO and Fukui function analysis of 5-methoxy-1H-benzo[d]imidazole-2(3H)-thione by DFT studies. J Mol Struct 1130:511–521View ArticleGoogle Scholar
- Obayes H, Alwan G, Al-Amiery A, Kadhum A, Mohamad A (2013) Thermodynamic and theoretical study of the preparation of new buckyballs from corannulene, coronene, and circulene. J Nanomater 2013;8. Article ID 451920Google Scholar
- Sastri VS (1998) Green corrosion inhibitors. Theory and practice. Wiley, HobokenGoogle Scholar
- Olivares-Xometl O, Likhanova NV, Gomez B, Navarrete J, Llanos-Serrano ME, Arce E, Hallen JM (2006) Electrochemical and XPS studies of decylamides of alpha-amino acids adsorption on carbon steel in acidic environment. Appl Surf Sci 252(6):2894–2909View ArticleGoogle Scholar
- Al-Azawi K, Al-Baghdadi S, Mohamed A, Al-Amiery A, Abed TK, Mohammed SA, Kadhum AA, Mohamad AB (2016) Synthesis, inhibition effects and quantum chemical studies of a novel coumarin derivative on the corrosion of mild steel in a hydrochloric acid solution. Chem Cent J 10(1):23View ArticleGoogle Scholar
- Likhanova NV, Martيnez-Palou R, Veloz MA, Matيas DJ, Reyes-Cruz VE, OlivaresXometl O (2007) Microwave-assisted synthesis of 2-(2-pyridyl)azoles. Study of their corrosion inhibiting properties. J Heterocycl Chem 44(1):145–153View ArticleGoogle Scholar
- Chen G, Zhang M, Zhao I, Zhou R, Meng Z, Zhang J (2013) Investigation of ginkgo biloba leave extracts as corrosion and oil field microorganism inhibitors. Chem Cent J 7:83View ArticleGoogle Scholar
- Fomina L, Porta B, Acosta A, Fomine S (2000) Novel substituted 1-amino-4,5,8-naphthalenetricarboxylic acid-1,8-lactam-4,5-imides: experimental and theoretical study. J Phys Org Chem 13:705–712View ArticleGoogle Scholar
- Lukovits I, Kalman E, Zucchi F (2001) Corrosion inhibitors—correlation between electronic structure and efficiency. Corrosion 57:3–8View ArticleGoogle Scholar
- Obayes R, Al-Amiery A, Alwan G, Alobaidy A, Al-Amiery A, Kadhum A, Mohamad A (2014) Quantum chemical assessment of benzimidazole derivatives as corrosion Inhibitors. Chem Cent J 8(21):1–8Google Scholar
- Obayes R, Al-Amiery A, Alwan G, Abdullah T, Kadhum A, Mohamad A (2017) Sulphonamides as corrosion inhibitor: experimental and DFT studies. J Mol Struct 1138:27–34View ArticleGoogle Scholar